View stunning SlideShares in full-screen with the new iOS app!Introducing SlideShare for AndroidExplore all your favorite topics in the SlideShare appGet the SlideShare app to Save for Later — even offline
View stunning SlideShares in full-screen with the new Android app!View stunning SlideShares in full-screen with the new iOS app!
Fatigue of Aircraft StructuresVol. 1 (2011) 53-5610.2478/v10164-010-0037-3 ANALYSIS OF THE POSSIBILITY TO ASSESS THE OCCURRENCE OF HIDDEN CORROSION IN LAP JOINTS USING ACTIVE THERMOGRAPHY Lukasz Kornas Krzysztof Dragan Air Force Institute of Technology, Warsaw, Poland Abstract The article details the NDT technique of pulse thermography used for objective diagnosis ofriveted lap joints construction. The degradation of materials manifesting in corrosion is inherentin the process of aircraft operation. One type of corrosion is galvanic corrosion occurring in theoverlap joints (known as hidden corrosion). As a result of the potential difference between the twolayers of the aluminum alloy skin, there occurs the phenomenon of oxidation of the material,producing corrosion products in the form of oxide compounds characterized by heat propertiesdifferent than those of the base material. Active thermography techniques allow observing infraredenergy, which changes due to the difference of thermal properties of the tested materials.1. INTRODUCTION Corrosivity is a very important phenomenon unfavourably affecting materials used in aviation.Corrosivity necessitates continuous aircraft surveillance during operation. The effect of corrosionprocesses is the damage of the material observed mainly on the surface of the material in the formof an accumulation of solid compounds such as oxides, rust and scale resulting from chemicalreactions. These chemical reactions are caused by changing weather conditions, increasedhumidity and the working environment such as contact with sea water. In many cases, the aircraftstructural component exposed to corrosion is the plated area of the lap riveted joints. As a result ofthe difference in potential at the interface between two materials, oxidation of the material occurscreating corrosion products in the form of metal oxides. In the case of aircraft structures made oflight alloys (usually aluminium alloys), these are mostly aluminium oxides Al2O2*3H2O, whosemolar volume is greater than that of pure aluminium. They accumulate between adjacent materials,causing local surface deformations. Continuous process of creating metal oxide contributes tofatigue. Ignoring this phenomenon may lead to deterioration in strength properties of joinedmaterials as well as damage of the rivet connecting them. It is a kind of hidden corrosion calledpillowing. Unauthenticated | 126.96.36.199 Download Date | 11/28/12 2:01 PM
Analysis of the Possibility to Assess the Occurrence of Hidden Corrosion in Lap Joints Using Active Thermography Fig. 1. Hidden corrosion (pillowing), the result of test with the use of DAIS system The DAIS system measures the degree of surface deformation caused by the presence of solidmetal compounds at the boundary between two materials. Using a number of different testtechniques enables better verification of the research results. The authors used a pulsedthermography technique, which allows the registration of changes in infrared radiation emitted bythe material. Based on the fundamental thermal coefficients (table. 1) for specific materials, theauthors conducted preliminary tests to confirm the presented thesis. Table 1. Basic thermophysical properties of selected materials.2. TEST RESULTS While performing preliminary tests, samples with the damaged anti-corrosion coating from thewing flap of Su-22 aircraft were used (Fig.2). The tests were carried out with pulsed thermographyusing EchoTherm. Hidden corrosion can manifest itself through the paint coating damage such ascracks, blowholes, etc. This causes the varnish layer flaking due to lack of adhesion to the surface.Anti-corrosion coating damage is caused by adverse external factors such as humidity, exposure tosea water or by contaminants introduced during the production stage. Thermographic results of thedamaged paint coating are shown on the thermograph below (Fig. 2). 54 Unauthenticated | 188.8.131.52 Download Date | 11/28/12 2:01 PM
Łukasz Kornas, Krzysztof Dragan Fig.2. a) damaged anti-corrosion paint coating, b) thermograph of damaged anti-corrosion paint coating Hidden corrosion manifests itself mostly as a result of the material oxidation creating solidoxide compounds. In aircraft structures, because of the materials used in the plating, corrosionproducts are aluminium oxides. The resulting compounds are characterized by other thermalproperties allowing their detection with thermographic methods. Preliminary tests were carried outon the object with riveted joints. Solids with other thermal parameters in relation to the basematerial (aluminium alloy) were introduced to lap joints. They cause disruption in homogenousintensity of infrared radiation emission on the surface of the tested object. The thermograph of thesample tested and the diagram illustrating the surface intensity of infrared radiation during coolingof the material are presented below (Fig.3). Fig.3. Thermograph of the sample tested and the diagram illustrating the surface intensity 55 Unauthenticated | 184.108.40.206 Download Date | 11/28/12 2:01 PM
Analysis of the Possibility to Assess the Occurrence of Hidden Corrosion in Lap Joints Using Active Thermography3. SUMMARY Preliminary results with the pulsed thermography method show the capabilities of the selectedtechnique for hidden corrosion evaluation in aircraft structures. With the method used we caneasily and quickly check the quality and correctness of paint coating at the stage of application, aswell as its status during operation (Fig. 2). The infrared technique offers opportunities fordetecting material inclusions due to differences in thermal properties. With this technique adifferent infrared radiation wavelength is detected in the area where material compounds ofdifferent thermal parameters are present (Fig. 3).REFERENCES Dragan, K. & Klimaszewski, S. (2003). Rozpoznanie i klasyfikacja korozji ukrytej w konstrukcji statków powietrznych za pomocą systemu DAIS. 32 Krajowa Konferencja Badań Niszczących, 27-30.10.2003 Międzyzdroje. Oliferuk, W. (2008). Termografia podczerwieni w nieniszczących badaniach materiałów i urządzeń. Warszawa: Biuro Gamma. Świderski, W. (2010). Metody termograficzne w nieniszczących badaniach materiałów kompozytowych do zastosowania specjalnych. Wojskowy Instytut Techniczny Uzbrojenia, Zielonka. Matzkanin, G.A. & Yolken, H.T. (2007). Nondestructive Evaluation Techniques for Detecting Hidden Corrosion, The AMMTIAC Quarterly. 2(2), 3-6. Vavilov, V.R. (2003). Non-contact one-sided evaluation of hidden corrosion in metallic constructions by using transient infrared thermography. Revista de Metalurgia. (2003), 235- 242. Perez, I. & Kulowitch, P. Thermography for characteriziation of corrosion damage. Naval Air Warfare Center, Aircraft Division Patuxent River MD 20670. Shepard, S.M. (2001). Thermographic Detection of Front and Back Surface Corrosion. Thermal Wave Imaging, Inc. Ferndale, MI 48220. 56 Unauthenticated | 220.127.116.11 Download Date | 11/28/12 2:01 PM